| ||Format||Pages||Price|| |
|7||$42.00||  ADD TO CART|
|Hardcopy (shipping and handling)||7||$42.00||  ADD TO CART|
|Standard + Redline PDF Bundle||14||$50.40||  ADD TO CART|
Significance and Use
This test method is intended to determine the volume distribution of pores in catalysts and catalyst carriers with respect to the apparent diameter of the entrances to the pores. In general, both the size and volume of pores in a catalyst affect its performance. Thus, the pore volume distribution is useful in understanding a catalyst's performance and in specifying a catalyst that can be expected to perform in a desired manner.
1.1 This test method covers the determination of the pore volume distributions of catalysts and catalyst carriers by the method of mercury intrusion porosimetry. The range of apparent diameters of pores for which it is applicable is fixed by the operant pressure range of the testing instrument. This range is typically between apparent pore entrance diameters of about 100 and 0.003 μm (3 nm).
1.2 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.4 This standard does not purport to address all of the safety problems, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. Specific hazard information is given in Section 8.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E177 Practice for Use of the Terms Precision and Bias in ASTM Test Methods
E456 Terminology Relating to Quality and Statistics
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
ICS Number Code 71.040.30 (Chemical reagents)